6. Single molecule analysis of DNA nanotube polymerization
6.4.3. Comparison with previously reported reaction rates of DNA self-
Inferred association rate constant
In section 6.3.2, we measured kon to be (5.99±0.15) ×105 /M/sec for the polymerization
model. In kTAM, the inferred association rate constant for a single DNA tile binding to an available site at the end of a DNA nanotube ksiteon was expected to be ≈ 2×kon =
2×(5.99±0.15)×105/M/sec. The inferredksiteon fell within the same order of magnitude as the previously reported forward rate measurements involving DNA hybridization [QW89,
GT81,WF91,MS93], and from numerical analysis of tile-based DNA self-assembly [ZW09]. Quartin and Wetmur [QW89] showed that the association reaction of a simple interaction between two short DNA strands is diffusion limited and determinedkon to be on the order
of 6×105/M/sec. From a series of DNA toehold exchange experiments, Zhang and Winfree obtained the range of forward rate to be (1−6)×106 /M/sec [ZW09].
The most comparable analysis of DNA self-assembly to the DNA nanotube polymeriza- tion reported here, is the kinetic Monte Carlo simulation of DNA ribbon growth done by Chen et al [CSGW07]. However, their kinetic parameter measurement was indirect. To obtain agreement between their AFM observation of assembly data and their simulations, Chen et al chose the forward rate ksiteon to be 17×106 /M/sec, which is 14× faster than our measurement. Given the sensitivity of their simulation results to the two adjustable parameters, namelykonsiteand the free energy of sticky-end interaction ∆G◦, it is likely that their inference ofksiteon value had significant uncertainty, which was not explicitly stated in the manuscript. In two separate works with different types of DNA ribbon, Schulman and Winfree [SW07] as well as Fujibayashi and Murata [FM09] used 106 /M/sec as the typical association rate constant in their analysis and found the number reasonable.
To evaluate the inferred thermodynamic parameters of our measurement, we compared the enthalpy and entropy values to theoretical predictions and to values from previously reported studies of the free energy of DNA hybridization. Both inferred enthalpy and entropy values are very close to the theoretical estimates used in the original presentation of the kTAM paper [Win98]. In that framework, the expected enthalpy of disassembly was calculated to be ∆H◦ =R×sb×(4000 K), where s is the number of base pairs in a
sticky end andb is the number of sticky end bonds. For b=2, s=6, the simple expression yielded the value of ∆H◦ = 95 kcal/mol, which is within 10% of our measurement of ∆H◦ = 87.9±2.0 kcal/mol. For the entropy, using the kTAM, α=ln(20) [Win98], the theoretical value was predicted to be ∆S◦ = R×(11sb+α) = 0.268 kcal/mol/K, which is within 10% of the measured ∆S◦ = 0.251±0.006 kcal/mol/K in our experiment. Finally, our inferred values of ∆H◦’s and ∆S◦’s, we calculated the standard free energy of two sticky end interactions at 37 ◦C to be ∆G◦37◦C = ∆H◦ −T37◦C∆S◦ = 12.2 kcal/mol and 9.5 kcal/mol for the values based on kTAM and our experiment, respectively. The ∆G◦37◦C from kTAM is within 30% difference from our measured ∆G◦37◦C.
To the best of our knowledge, the only published values for thermodynamic parameters of double crossover tile-based DNA structures in solution were obtained from bulk studies of DNA ribbons of designed widths [SW07]. The ribbons of different widths were composed of multiple tiles with 5 bp sticky ends, which is shorter than the 6 bp sticky ends in our tiles. Schulman and Winfree extracted ∆H◦ and ∆S◦ from a series of UV absorbance data by employing van’t Hoff analysis. They measured ∆H◦= 102.4 kcal/mol and ∆S◦ = 0.300 kcal/mol/K. To account for their shorter sticky ends, we multiplied these values by 6/5, which is the ratio of sticky end lengths of our DNA nanotube and Shulman and Winfree’s ribbon, which gives ∆H◦ = 122.9 kcal/mol and ∆S◦ = 0.360 kcal/mol/K. Their adjusted values of ∆H◦ and ∆S◦ are within 45% and 22% of our measurement, respectively. Using these adjusted ∆H◦’s and ∆S◦ values, we calculated ∆G◦37◦C = 11.3 kcal/mol, which is within 18% of our measured ∆G◦37◦C.
The thermodynamic parameters of DNA hybridization depend strongly on the DNA se- quences and buffer condition, which could explain the difference of as much as 45% between our measurements and the thermodynamic values obtained by Schulman and Winfree. Moreover, the inter- and intra-monomer strain between DNA ribbons and DNA nanotubes are likely to be different. Their publishedn-tile-wide ribbons assembled from 2(n-2) unique single tile and two double tiles, each have different sticky end sequences compared to the tile used in this work. In addition, their thermodynamic measurements were acquired in the absence of crowding agent and in 12.5 mM concentration of Magnesium, compared to 10 mM in our polymerization buffer.
Furthermore, the measured thermodynamic values are also not incompatible with Nang- reaveet al.’s van’t Hoff analysis of their FRET measurement of quadruple-crossover (QX) molecules [NYL09]. The QX molecule, in essence, is a flat sheet of 4 parallel DNA helices. By attaching different 6 bp sticky ends to a QX pair, the thermodynamic properties of dif-
ferent configurations of sticky ends were extensively studied. The relevant subset of their experiments is the measurement of the interaction between 2 pairs of sticky ends that are located adjacent to each other. In the two variants that they constructed, the enthalpy was measured to be 105.1±7.8 kcal/mol and 116.6±19 kcal/mol. For the entropy of the reaction, they determined the values to be 0.301±0.025 kcal/mol/K and 0.334±0.057 kcal/mol/K. These values are within a range that is less than 36% of our measurement.
Another relevant value to compute is the expected melting temperatureTmof DNA nan-
otubes in Kelvin. From simple thermodynamics, the melting temperature can be calculated as
Using the theoretical values from kTAM [Win98], the melting temperature for a reaction with 100 nM, 200 nM, 300 nM, 400 nM, and 500 nM free tile concentration is calculated to be 43.5◦C, 44.9◦C, 45.7◦C, 46.4◦C, and 46.9◦C , respectively. The calculated values are less than 8 ◦C higher than the measured equilibrium temperature in the polymerization rate vs. temperature plots (Fig. 6.7), which is in close agreement with our measurement and predictions based on a simple model. Similarly, the discrepancy inTm is likely because
the kTAM number is derived from a simple model and ignores the sequence dependence of ∆H◦ and ∆S◦. Nonetheless, this close agreement illustrates the usefulness of the simple energetics model in the kTAM for estimating thermodynamic values in DNA self-assembly.